Chemical bonding and elastic properties of quaternary arsenide oxides YZnAsO and LaZnAsO investigated by first principles
SHI Yiming 1, YE Shaolong 2 1. Department of Basic Teaching, Hunan Institute of Technology, Hengyang 421000, China; 2. School of Metallurgical Science and Engineering, Central South University, Changsha 410083, China Received 9 March 2011; accepted 8 June 2011
Abstract: The structural parameters, chemical bonding and elastic properties of the tetragonal phase quaternary arsenide oxides YZnAsO and LaZnAsO were investigated by using densityfunctional theory (DFT) within generalized gradient approximation (GGA). The GGA calculated structural parameters are in agreement with the experimental results. Population analysis suggests that the chemical bonding in YZnAsO and LaZnAsO can be classified as a mixture of ionic and covalent characteristic. Singlecrystal elastic constants were calculated and the polycrystalline elastic modules were estimated according to Voigt, Reuss and Hill’s approximations (VRH). The result shows that both YZnAsO and LaZnAsO are relatively soft materials exhibiting ductile behavior. The calculated polycrystalline elastic anisotropy result shows that LaZnAsO is more anisotropy in compressibility and YZnAsO is more anisotropy in shear. Key words: YZnAsO; LaZnAsO; chemical bonding; elastic properties; densityfunctional theory; generalized gradient approximation; Voigt, Reuss and Hill’s approximations
temperature. The positive Seebeck coefficients of the 1 Introduction epitaxial film indicated a ptype semiconductor. The optical bandgap of LaZnAsO was estimated to be about The quaternary oxypnictide layered compounds 1.5 eV. It is expected that LaZnAsO may be a promising REZnPO (RE=Y, La−Nd, Sm, Gd, Dy, Ho) and matrix for diluted magnetic semiconductors if Zn 2+ is REZnAsO (RE=Y, La−Nd, Sm, Gd−Er) with the partially replaced by a divalent transition metal, such as ZrCuSiAstype structure have received considerable Mn 2+ . LINCKE et al  have synthesized well attention [1−6] because of the discovery of crystallized form REZnAsO (RE = Y, La) from the superconductivity in LaOFeP, LaNiOP and ingots of rare earth elements, arsenic, and ZnO in LaFeAsO(F)[7−11]. They have similar layered structures NaCl/KCl fluxes in sealed silica ampoules. The with alternating [ReO] and [ZnPn] (Pn=As, P) layers, REZnAsO structures consist of alternate stacks of and exhibit a wide variety of interesting electrical, (RE 3+ O 2− ) and (Zn 2+ As 3− ) layers with covalent RE—O optical, and magnetic properties. YZnAsO and LaZnAsO, and Zn—As intralayer and weak ionic interlayer bonding. which are isostructural to the layered rareearth LaZnAsO and YZnAsO show an optical bandgap of oxypnictides REZnAsO (RE=Y, La−Nd, Sm, Gd, Er), Eg≈2.3 eV and Eg≈1.9 eV respectively. BANNIKOV et are semiconductor compounds with band gap of 1.5−2.3 al  investigated the electronic properties and chemical eV in experimental investigation [2, 5] or 0.65−1.3 eV in bonding picture of LaZnAsO and YZnAsO. The band theoretical calculation . KAYANUMA et al  have structures result showed that both of them are successfully grown LaZnAsO thin films on MgO semiconductors with the band gaps of about 0.65 eV for substrates with an epitaxial relationship of (001) LaZnAsO and 1.3 eV for YZnAsO. The bonding can be LaZnAsO || (001) MgO and  LaZnAsO ||  classified as a mixture of ionic and covalent MgO. The electrical conductivity of the undoped contributions. To the best of our knowledge, there are LaZnAsO epitaxial films was 0.2 S/cm at room no reports on the elastic properties of YZnAsO and
Foundation item: Project (50474051) supported by the National Natural Science Foundation of China Corresponding author: SHI Yimin; Tel: +8615111157635; Email: [email protected] DOI: 10.1016/S10036326(11)608698 SHI Yiming, et al/Trans. Nonferrous Met. Soc. China 21(2011) 1378−1382 1379
LaZnAsO. However, elastic properties are very site (1/4, 1/4, zY/La), O at 2a site (3/4, 1/4, 0), Zn at 2b important for materials because they provide information site (3/4, 1/4, 1/2), and As at 2c site (1/4, 1/4, zAs) [2, on interatomic potentials and relate to various 5−6], in which zY/La and zAs are the internal coordinates fundamental solid state phenomena such as interatomic of Y/La and As, respectively. The experimental lattice bonding, equations of state, phonon spectra as well as parameters are a=b=0.394 2 nm and c=0.884 0 nm for specific heat capacity, thermal expansion, Debye YZnAsO, and a=b=0.409 6 nm and c=0.907 0 nm for temperature . Most importantly, elastic properties are LaZnAsO; and the internal coordinates of Y/La and essential for many practical applications related to the As are reported as zY/La=0.121 7 and zAs=0.682 5 for mechanical properties of solid: load deflection, internal YZnAsO and zY/La=0.1337 and zAs=0.6711 for LaZnAsO strain, thermoelastic stress, sound velocities and fracture [2, 5−6], respectively. toughness . In this study, the chemical bonding and elastic properties of the tetragonal phase of YZnAsO and LaZnAsO are investigated using first principles calculations based on DFT.
2 Calculation details and models
The first principle calculations were based on DFT using a planwave expansion of the wave function implanted in CASTEP code . The exchange correlation energy was calculated by the GGA with the PerdewBurkeErnzerhof (PBE) function . The ionic cores were represented by normconserving pseudo potentials [15−17] for Y, La, O, Zn and As atoms. The Y 4d 15s 2 electrons, La 5d 16s 2 electrons, O 2s2 2p 4 electrons, Zn 3d 104s 2 electrons, and As 4s 24p 3 electrons were Fig. 1 Crystal structure sketch of YZnAsO explicitly treated as valence electrons. The Monkhorst and Pack scheme of kpoint sampling was used for At the first stage the full structural optimization of integration over the first Brillouin zone . The cutoff this phase was performed both over the lattice energy was chosen to be 900 eV, and the Brillouinzone parameters and the atomic positions including the sampling kpoint set mesh parameters were 12×12×6. internal coordinate zY/La and zAs. The calculated This set of parameters assure the total energy optimization lattice parameters a, c, V and atomic convergence of 5.0×10 −6 eV/atom, the maximum force of coordinates compared with available experimental data 0.01 eV/Å, the maximum stress of 0.02 GPa and the [2, 5] for YZnAsO and LaZnAsO are summarized in maximum displacement of 5.0×10 −4 Å. Table 1, which show that the calculated structural parameters are in agreement with the experimental data. 3 Results and discussion 3.2 Chemical bonding 3.1 Geometry and structure properties The Mulliken bond population is useful for The crystal structure of the tetragonal phase of evaluating the bonding character in a material. A high YZnAsO and LaZnAsO belongs to the space group value of the bond population indicates a covalent bond, P4/nmm, Z=2 (ZrCuSiAs type), where blocks [YO/LaO] and a low value indicates an ionic bond. Positive and are sandwiched with [ZnAs] blocks as depicted in Fig. 1. negative values indicate bonding and antibonding There are four inequivalent atomic positions: Y/La at 2c states, respectively [17, 19]. The Mulliken atomic
Table 1 Calculated lattice parameters and atomic internal coordinate compared with experimental data [2, 5] for YZnAsO and LaZnAsO 3 Compound Method a/nm c/nm V/nm zY/La zAs Experiment 0.394 2 0.884 0 0.137 4 0.121 7 0.682 5 YZnAsO Calculation 0.396 3 0.885 8 0.139 1 0.119 5 0.693 4 Experiment 0.409 6 0.907 0 0.152 1 0.133 7 0.671 1 LaZnAsO Calculation 0.400 1 0.899 0 0.143 9 0.123 0 0.683 0 1380 SHI Yiming, et al/Trans. Nonferrous Met. Soc. China 21(2011) 1378−1382 population analyses of YZnAsO and LaZnAsO listed in Table 4 Calculated single crystal elastic constants Cij, bulk Tables 2 and 3 show a charge transfer from [YO/LaO] modulus B and compressibility coefficient β of YZnAsO and block to [ZnAs] block, indicating that the internal of LaZnAsO
[YO/LaO] block and the [ZnAs] block is ionic character; Compound C11 C33 C44 C66 — and the bond population shows the intrablock of Y O/ YZnAsO 189.96 116.55 13.86 37.42 La—O and Zn—As are covalent character. The chemical LaZnAsO 227.57 112.33 35.05 50.32 bondings in YZnAsO and LaZnAsO have a mixture of ionic and covalent characteristic, which is in agreement Compound C12 C13 B/GPa β with the results of Refs. [5−6]. YZnAsO 36.91 41.79 78.38 0.012 76 LaZnAsO 37.18 53.10 87.00 0.011 49 Table 2 Mulliken atomic population analysis of YZnAsO and LaZnAsO From Table 4, it can be seen that these criteria are Population Compound Species Charge/e all satisfied, which indicates that YZnAsO and LaZnAsO s p d Total are mechanically stable. The single crystal bulk moduli B Y 0.41 0.26 1.47 2.14 0.86 are 78.38 and 87.00 GPa for YZnAsO and LaZnAsO, O 1.84 4.89 0.00 6.72 −0.72 respectively, which means that YZnAsO and LaZnAsO YZnAsO Zn 0.67 1.34 9.96 11.98 0.02 are soft materials. The polycrystal bulk modulus B and shear modulus G are estimated using the VRH approach As 1.35 3.80 0.00 5.15 −0.15 in the following forms [20−23]: La 0.22 0.12 1.46 1.79 1.21 B = (2C + 2C + C + 4C ) /9 , O 1.87 4.91 0.00 6.78 −0.78 V 11 12 33 13 LaZnAsO Zn 0.73 1.38 9.96 12.08 −0.08 GV = (M + 3C11 − 3C12 +12C44 + 6C6 6 ) / 30 , As 1.49 3.87 0.00 5.35 −0.35 2 BR = C / M ,
2 Table 3 Mulliken bond population analysis of YZnAsO and GR = 15 /[18BV / C + 6 /(C11 − C12 ) + 6 / C44 ) + 3 / C 66 ] ,
LaZnAsO 2 2 C = (C11 + C12 )C33 − 2C 1 3 , Compound Bond Population Length/nm Y—O 0.77 0.224 623 M = C11 + C12 + 2C33 − 4C 1 3 , Zn—AS 0.33 0.261 935 B = ( B + B ) / 2 , YZnAsO H R V Zn—Zn 0.88 0.280 202 G H = (G R + GV ) / 2 (2) O—O −0.10 0.280 202 The elastic modulus E and Poisson ratio v are La—O 0.54 0.226 381 estimated by [20−21] Zn—As 0.39 0.260 921 LaZnAsO Zn—Zn 0.75 0.282 911 E = 9BG /(3B + G ) , O—O −0.08 0.282 911 ν = (3B − E) / 6B = (3B − 2G) /(6B + 2G ) (3)
3.3 Elastic properties All the calculated results are presented in Table 5. It Elastic constants are defined by means of a Taylor can be seen that the value of BH/GH ratio for YZnAsO is expansion of the total energy, namely, the derivative of 2.57 and for LaZnAsO is 1.87, which are larger than the critical value (1.75) separating ductile and brittle the energy as a function of a lattice strain . The materials [20−21], indicating that both YZnAsO and tetragonal phase YZnAsO and LaZnAsO crystals have LaZnAsO behave in a ductile manner, and YZnAsO is six independent elastic constants C11, C33, C44, C66, C12 more ductile than LaZnAsO. It is known that the values and C [20−21] which are presented in Table 4. For the 13 of the Poisson ratio (ν) are minimal for covalent tetragonal crystal, its mechanical stability requires that materials (ν=0.1), and increase for ionic systems [20−21]. its independent elastic constants should satisfy the Born’s In our case, the calculated Poisson ratios (ν) are 0.327 7 stability criteria [20−21]: for YZnAsO and 0.272 9 for LaZnAsO, which means a Cii>0 (i=1, 3, 4, 6), sizable ionic contribution in intrabonding. The elastic anisotropy in compressibility (A ) C11−C12>0, C11+C33−2C13>0, B and shear (AG) using the model in Ref.  for 2(C +C )+C +4C >0 (1) 11 12 33 13 polycrystalline materials is SHI Yiming, et al/Trans. Nonferrous Met. Soc. China 21(2011) 1378−1382 1381 Table 5 Calculated polycrystalline elastic constants, elastic that LaZnAsO is more anisotropy in compressibility and modulus E, Poisson ratio ν and BH/GH of YZnAsO and YZnAsO is more anisotropy in shear. LaZnAsO
Compound BV BR BH GV GR References YZnAsO 81.94 78.38 80.16 38.09 24.33  KAYANUMA K, HIRAMATSU H, HIRANO M, KAWAMURA R, LaZnAsO 94.91 87.00 90.96 52.36 45.02 YANAGI H, KAMIYA T, HOSONO H. Apparent bipolarity and seebeck sign inversion in layered semiconductor: LaZnOP [J]. Phys Compound G B /G E/GPa ν H H H Rev B, 2007, 76: 195325. YZnAsO 31.21 2.57 82.87 0.327 7  KAYANUMA K, KAWAMURA R, HIRAMATSU H, YANAGI H, HIRANO M, KAMIYA T, HOSONO H. Heteroepitaxial growth of LaZnAsO 48.69 1.87 123.95 0.272 9 layered semiconductors, LaZnOPn (Pn=P and As) [J]. Thin Solid Films, 2008, 516: 5800−5804.  TAKANO Y, KOMATSUZAKI S, KOMASAKI H, WATANABE T, AB = (BV − BR ) /(BV + BR ) , TAKAHASHI Y, TAKASE K. Electrical and magnetic properties of A = (G − G ) /(G + G ) (4) G V R V R LnOZnPn (Ln = rare earths; Pn = P, As, Sb) [J]. J Alloys Compd, A value of zero represents elastic isotropy and a 2008, 451: 467−469.  LINCKE H, GLAUM R, DITTRICH V, TEGEL M, JOHRENDT D, value of 100% is the largest possible anisotropy. The HERMES W, MÖLLER M H, NILGES T, PÖTTGEN R. Magnetic, calculated polycrystalline elastic anisotropy in bulk optical, and electronic properties of the phosphide oxides REZnPO modulus AB and shear modulus AG are listed in Table 6. (RE = Y, LaNd, Sm, Gd, Dy, Ho) [J]. Z Anorg Allg Chem, 2008, 634, 1339−1348. It shows that the shear modulus anisotropy AG is larger  LINCKE H, GLAUM R, DITTRICH V, MÖLLER M H, PÖTTGEN than the bulk modulus anisotropy A for both YZnAsO B R. Structure and optical properties of the arsenide oxides REZnAsO and LaZnAsO. And LaZnAsO is more anisotropy in (RE=Y, La−Nd, Sm, Gd−Er) [J]. Z Anorg Allg Chem, 2009, 635: compressibility (4.35%) and YZnAsO is more anisotropy 936−941. in shear (22.04%). The larger anisotropy may produce  BANNIKOV V V, SHEIN I R, IVANOVSKII A L. Electronic cracking propagation during sample preparing and using. properties and chemical bonding in quaternary arsenide oxides LaZnAsO and YZnAsO [J]. Mater Chem Phys, 2009, 116: 129−133. Utilization of very small YZnAsO and LaZnAsO  KAMIHARA Y, HIRAMATSU H, HIRANO M, KAWAMURA R, particles would be a way of minimizing cracking. YANAGI H, KAMIYA T, HOSONO H. Ironbased layered superconductor: LaOFeP [J]. J Am Chem Soc, 2006, 128: Table 6 Calculated polycrystalline elastic anisotropy for bulk 10012−10013.  WATANABE T, YANAGI H, KAMIYA T, KAMIHARA Y, modulus A and shear modulus A of YZnAsO and LaZnAsO B G HIRAMATSU H, HIRANO M, HOSONO H. Nickelbased Compound AB/% AG/% oxyphosphide superconductor with a layered crystal structure, LaNiOP [J]. Inorganic Chemistry, 2007, 46(19): 7719−7722. YZnAsO 2.22 22.04  KAMIHARA Y, WATANABE T, HIRANO M, HOSONO H.
LaZnAsO 4.35 7.54 Ironbased layered superconductor La[O1−xFx]FeAs (x= 0.05−0.12)
with Tc=26 K [J]. J Am Chem Soc, 2008, 130: 3296−3297.  WEN H H. Developments and perspectives of ironbased 4 Conclusions hightemperature superconductors [J]. Adv Mater, 2008, 20(19): 3764−3775.  REN Z A, ZHAO Z X. Research and prospects of ironbased 1) The structural parameters, chemical bonding and superconductors [J]. Adv Mater, 2009, 21(45): 4584−4593. elastic properties of YZnAsO and LaZnAsO were  PENG F, CHEN D, YANG X D. Firstprinciples calculations on investigated by first principles. The GGA calculated elasticity of OsN2 under pressure [J]. Solid State Commun, 2009, 149: structural parameters are in agreement with the available 2135−2138. experimental data.  SEGALL M D, LINDAN PHILIP J D, PROBERT M J, PICKARD C J, HASNIP P J, CLARK S J, PAYNE M C. Firstprinciples 2) The chemical bonding was analyzed. The results simulation: Ideas, illustrations and the CASTEP code [J]. J Phys: show that YZnAsO and LaZnAsO are a mixture of ionic Condens Matter, 2002, 14(11): 2717−2744. and covalent characteristic.  PERDEW J P, BURKE K, ERNZERHOF M. Generalized gradient 3) The single crystal elastic constants were approximation made simple [J]. Phys Rev Lett, 1996, 77: 3865−3868. calculated, and the polycrystal bulks and shear modulus,  HAMANN D R, SCHLUTER M, CHIANG C. Normconserving elastic modulus, Poisson ratios and BH/GH were derived. pseudopotentials [J]. Phys Rev Lett, 1979, 43: 1494−1497. The results show that both YZnAsO and LaZnAsO are  ZHANG X Y, CHEN Z W, ZHANG S L, LIU R P, ZONG H T, mechanically stable and relatively soft materials JING Q, LI G, MA M Z, WANG W K. Electronic and optical behaving in a ductile manner. properties of rocksalt aluminum nitride obtained from first principles [J]. J Phys: Condens Matter, 2007, 19: 425231. 4) The calculated polycrystalline elastic anisotropy  XIA Q L, YI J H, LI Y F, PENG Y D, WANG H Z, ZHOU C S. in bulk modulus and anisotropy in shear modulus show Firstprinciples investigations of the band structure and optical 1382 SHI Yiming, et al/Trans. Nonferrous Met. Soc. China 21(2011) 1378−1382
properties of γboron [J]. Solid State Commun, 2010, 150: 605−608. bonding in ternary arsenide SrFe2As2 and quaternary oxyarsenide  MONKHORST H J, PACK J D. Special points for brillouinzone LaFeAsO—Basic phases for new 38−55 K superconductors from integrations [J]. Phys Rev B, 1976, 13: 5188−5192. first principles [J]. Physica C, 2009, 469: 15−19.  HERMET P, GOUMRISAID S, KANOUN M B, HENRARD L.  HILL R. The elastic behaviour of a crystalline aggregate [J]. Proc Firstprinciples investigation of the physical properties of magnesium Phys Soc London A, 1952, 65: 349−355. nitridoboride [J]. J Phys Chem C, 2009, 113: 4997−5003.  ANDERSON O L. A simplified method for calculating the Debye  SHEIN I R, IVANOVSKII A L. Elastic properties of quaternary temperature from elastic constants [J]. J Phys Chem Solids, 1963, oxyarsenide LaOFeAs and LaOFeP as basic phases for new 26−52 K 24(7): 909−917. superconducting materials from first principles [J]. Scripta Materialia,  CHUNG D H, BUESSEM W R. Anisotropy in single crystal 2008, 59: 1099−1102. refractory compounds, edited by vahldiek F W and mersol S A [M].  SHEIN I R, IVANOVSKII A L. Elastic properties and chemical Vol.2. New York: Plenum Press, 1968: 217.
四元砷氧化物 YZnAsO 和 LaZnAsO 的 化学键和弹性性质的第一性原理研究
施毅敏 1, 叶绍龙 2
1. 湖南工学院 基础教学部，衡阳 421000； 2. 中南大学 冶金科学与工程学院，长沙 410083
摘 要：利用基于密度泛函理论(DFT)的广义梯度近似(GGA)研究四方相四元砷氧化物 YZnAsO 和 LaZnAsO 的结 构参数、化学键和弹性性质。结果表明，GGA 计算的结构参数与实验值吻合较好。布居分析显示 YZnAsO 和 LaZnAsO 中的化学键具有混合的离子−共价特征。计算得到了单晶的弹性常数，由 Voigt, Reuss 和 Hill (VRH)近似 导出了多晶弹性模量，结果表明 YZnAsO 和 LaZnAsO 为具有一定延展性、相对较软的材料。多晶的弹性各向异 性结果显示，LaZnAsO 的体模量各向异性相对较大，而 YZnAsO 的剪切模量各向异性相对较大。 关键词：YZnAsO；LaZnAsO；化学键；弹性性质；密度泛函理论；广义梯度近似；VRH 近似 (Edited by YUAN Saiqian)